#------------------------------------------------------------------------------
#$Date: 2017-10-07 05:55:02 +0300 (Sat, 07 Oct 2017) $
#$Revision: 201844 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/04/44/7044427.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7044427
loop_
_publ_author_name
'Huang, Hui-Lin'
'Liu, You-Rong'
'Huang, Li-Hsun'
'Chiang, Ray-Kuang'
'Wang, Sue-Lein'
_publ_section_title
;
 Achiral Polyamine-Induced Chiral Zinc Gallophosphates with Fused Double
 Helix-Like Strands Exhibiting Blue to Green Photoluminescence
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C7DT02465G
_journal_year                    2017
_chemical_formula_sum            'C0.91 H3.19 Ga0.43 N0.57 O4 P Zn0.57'
_chemical_formula_weight         184.37
_chemical_name_common            ZG-5N-L
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      cubic
_space_group_IT_number           214
_space_group_name_Hall           'I 4bd 2c 3'
_space_group_name_H-M_alt        'I 41 3 2'
_symmetry_space_group_name_Hall  'I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I 41 3 2'
_audit_block_doi                 10.5517/ccdc.csd.cc1pd52b
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2017-09-20 deposited with the CCDC.
2017-10-04 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            48
_cell_length_a                   18.0228(13)
_cell_length_b                   18.0228(13)
_cell_length_c                   18.0228(13)
_cell_measurement_reflns_used    17342
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.303
_cell_measurement_theta_min      3.195
_cell_volume                     5854.2(7)
_computing_cell_refinement       'SAINT V8.34A (Bruker AXS Inc., 2013)'
_computing_data_collection       'APEX2 (Bruker AXS, 2010)'
_computing_data_reduction        'SAINT V8.34A (Bruker AXS Inc., 2013)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2008)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean 8.3333
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0314
_diffrn_reflns_av_unetI/netI     0.0159
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            27922
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.297
_diffrn_reflns_theta_min         1.598
_exptl_absorpt_coefficient_mu    5.528
_exptl_absorpt_correction_T_max  0.9485
_exptl_absorpt_correction_T_min  0.8345
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS V2014/2 (Bruker AXS Inc.)'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    2.510
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Cube
_exptl_crystal_F_000             4324
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.15
_platon_squeeze_details
;
The integral electron density in the voids is 683 electrons. The elctron density for N5C8H28 (protonated tetraethylenepentamine) calculated from the formula (N5C8H28)0.114(Zn0.57Ga0.43PO4) is 607 electrons.
;
_refine_diff_density_max         0.259
_refine_diff_density_min         -0.187
_refine_diff_density_rms         0.051
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.028(14)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     56
_refine_ls_number_reflns         1224
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.093
_refine_ls_R_factor_all          0.0158
_refine_ls_R_factor_gt           0.0147
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0193P)²+4.0977P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0397
_refine_ls_wR_factor_ref         0.0400
_reflns_Friedel_coverage         0.647
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                1188
_reflns_number_total             1224
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c7dt02465g2.cif
_cod_data_source_block           ZG-5N-L
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_original_cell_volume        5854.2(13)
_cod_database_code               7044427
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2014-3
_platon_squeeze_void_probe_radius 1.20
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'
'y+3/4, x+1/4, -z+1/4'
'-y+3/4, -x+3/4, -z+3/4'
'y+1/4, -x+1/4, z+3/4'
'-y+1/4, x+3/4, z+1/4'
'x+3/4, z+1/4, -y+1/4'
'-x+1/4, z+3/4, y+1/4'
'-x+3/4, -z+3/4, -y+3/4'
'x+1/4, -z+1/4, y+3/4'
'z+3/4, y+1/4, -x+1/4'
'z+1/4, -y+1/4, x+3/4'
'-z+1/4, y+3/4, x+1/4'
'-z+3/4, -y+3/4, -x+3/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-x+1/2, y+1, -z+1'
'x+1, -y+1, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1, -x+1, -y+1/2'
'-z+1, -x+1/2, y+1'
'-z+1/2, x+1, -y+1'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1, -x+1'
'y+1, -z+1, -x+1/2'
'-y+1, -z+1/2, x+1'
'y+5/4, x+3/4, -z+3/4'
'-y+5/4, -x+5/4, -z+5/4'
'y+3/4, -x+3/4, z+5/4'
'-y+3/4, x+5/4, z+3/4'
'x+5/4, z+3/4, -y+3/4'
'-x+3/4, z+5/4, y+3/4'
'-x+5/4, -z+5/4, -y+5/4'
'x+3/4, -z+3/4, y+5/4'
'z+5/4, y+3/4, -x+3/4'
'z+3/4, -y+3/4, x+5/4'
'-z+3/4, y+5/4, x+3/4'
'-z+5/4, -y+5/4, -x+5/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_occupancy
Ga1 Ga 0.25826(2) 0.34809(2) 0.11109(2) 0.01903(9) Uani 0.43 1 d P
Zn1 Zn 0.25826(2) 0.34809(2) 0.11109(2) 0.01903(9) Uani 0.57 1 d P
P1 P 0.38503(4) 0.24327(3) 0.15222(4) 0.01841(16) Uani 1 1 d .
O1 O 0.30388(10) 0.25416(11) 0.12949(12) 0.0292(4) Uani 1 1 d .
O2 O 0.22532(11) 0.39117(12) 0.20064(10) 0.0299(5) Uani 1 1 d .
O3 O 0.17376(11) 0.33856(11) 0.04786(11) 0.0268(4) Uani 1 1 d .
O4 O 0.32717(11) 0.41564(11) 0.06859(10) 0.0265(4) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Ga1 O4 106.67(9) . .
O2 Ga1 O3 107.25(9) . .
O4 Ga1 O3 109.77(9) . .
O2 Ga1 O1 110.58(9) . .
O4 Ga1 O1 110.88(8) . .
O3 Ga1 O1 111.53(9) . .
O2 P1 O1 111.34(12) 9 .
O2 P1 O3 111.64(12) 9 20_554
O1 P1 O3 107.25(12) . 20_554
O2 P1 O4 106.01(11) 9 42_544
O1 P1 O4 110.61(11) . 42_544
O3 P1 O4 110.04(12) 20_554 42_544
P1 O1 Ga1 124.80(12) . .
P1 O2 Ga1 132.15(13) 5 .
P1 O3 Ga1 125.73(13) 17_455 .
P1 O4 Ga1 122.99(12) 42_544 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ga1 O2 1.8868(19) .
Ga1 O4 1.900(2) .
Ga1 O3 1.9098(19) .
Ga1 O1 1.9110(19) .
P1 O2 1.529(2) 9
P1 O1 1.5315(19) .
P1 O3 1.534(2) 20_554
P1 O4 1.5380(19) 42_544
O2 P1 1.529(2) 5
O3 P1 1.534(2) 17_455
O4 P1 1.5380(19) 42_544
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.015 0.227 0.131 944 329 ' '
2 -0.020 0.223 0.616 990 354 ' '
